Comparative Evaluation of Antimicrobial Efficacy of Resin-Modified Glass Ionomers, Compomers and Giomers – An Invitro Study
P.Tarasingh1, J.Sharada Reddy2, K.Suhasini3, I.Hemachandrika4
ABSTRACT Background: Dental restorative materials, especially those applied in direct contact with the contaminated substrate, should have appropriate antibacterial activity in order to prevent residual bacteria from continuing their metabolic activity in addition to impairing new bacteria from reaching the toothrestoration interface. Aim: To determine the antibacterial efficacy of three different restorative materials against the common cariogenic microorganism i.e., Streptococcus mutans. Materials and Methods: Three different restorative materials were evaluated in this study: Giomer (Beautifil), Compomer (F2000) & Resin modified Glass ionomer (Fuji II LC) for their anti microbial efficacy against Streptococcus mutans by standard
agar diffusion method and zones of inhibition for each restorative material were calculated. Statistical Analysis: Inhibition zones around each restorative material were measured and values were subjected to one-way ANOVA with least square difference (LSD) Post-hoc test. Results: The mean inhibitory zones for Resin modified glass ionomers, Giomers & Compomers ranged from 10.1 – 6.90mm. Fuji II LC exhibited the highest mean inhibitory zone of 10.1 ± 1.97 for S.mutans. Beautifil exhibited mean inhibitory zone of 8.20 ± 1.62, whereas F2000 showed the least mean inhibitory zone of 6.90 ± 1.29. Conclusion: Based on the inhibitory zones of three restorative materials, Fuji II LC is recommended as the best restorative material among the three tested restorative materials.
Keywords: Antibacterial activity, Hybrid restorative materials, S. mutans
Introduction Dental caries is the most prevalent disease of mankind leading to early loss of teeth. The presence of micro-organisms in the oral cavity is one of the most important caries risk factors. Certain bacteria have been identified as more cariogenic than others among which the most important organism was Streptococcus mutans . Early attempts to control caries, involved techniques which removed sound tooth structure along with pits and fissures and then restored with restorative materials which do not have antimicrobial activity. Recurrent caries are lesions at the margin of existing restorations that become carious . Undesirable events such as pulp injury and pulp necrosis are frequently associated with the presence of residual bacteria after carious dentin removal and the ingress of new micro-organisms in the tooth-restoration interface as a result of micro leakage . In these procedures, restorative cements with antimicrobial properties are used in direct contact with residual carious tissue to promote the rehardening of the tissue and to reduce the viability of residual bacteria, thus preventing the occurrence of secondary caries. Besides antibacterial activity, such materials should also have good biocompatibility with the dentin-pulp complex . In the past, various dental cements were evaluated for their antimicrobial properties and it was found that this property is due to their low pH and due to release of fluoride ions from them. However, there is insufficient data regarding the fluoride release and low pH of recently used dental cements for their antimicrobial effect [4,5]. Glass ionomer cements are said to have excellent tooth bonding properties and also antimicrobial property but they are sensitive to moisture contamination, have low initial mechanical properties and inferior translucency. Hence, recently hybrid materials combining the technologies of glass-ionomers and composites were developed Journal of Clinical and Diagnostic Research. 2015 Jul, Vol-9(7): ZC85-ZC87
to overcome the above disadvantages of glass-ionomer cements. These hybrid materials mainly include Resin-modified Glass ionomer cement’s (RMGIC’s), Compomers (Polyacid-modified composites) & Giomers . As there is very little data regarding antimicrobial properties of hybrid restorative materials, this study was undertaken to evaluate the antimicrobial efficacy of three hybrid restorative materials viz., Fuji II LC (Resin-modified glass-ionomer), F2000 (compomer) and Beautifil (Giomer) against the Streptococcus mutans.
Materials and Methods This study was conducted at Dept. of Pedodontics with Preventive Dentistry, Govt. Dental College and Hospital, Hyderabad and Dept. of Microbiology, Institute of Preventive Medicine, Hyderabad in the year 2013.Three different light curing restorative materials, Giomer (Beautifil-II, Shofu Inc., Kyoto, Japan), F2000 (3M Dental Products, Hytac, ESPE) and Fuji II LC (GC Fuji II™ LC, GC Corporation, Tokyo) were used for the preparation of discs. A sterile hollow metal ring with 5mm inner diameter and 2mm thickness was used for the preparation of discs. Vaseline was applied as a separating media to the inner diameter of the ring. Beautifil and F2000 which are supplied in syringe form were flowed into the metal ring over a glass slab sandwiched between two mylar strips and light cured for 40 sec with halogen light curing unit and then removed from the ring to get the disc form. Fuji II LC is a powder-liquid system. Powder and liquid were mixed as per the manufacturer’s instructions, placed into the ring and light cured for 40 seconds. All the specimens were sterilized by autoclaving at 1210c at 15 lbs pressure for 15 min. Thus a total number of 30 discs (10 from each material) were prepared from three different restorative materials to test the antibacterial efficacy. 85
P. Tarasingh et al., Antimicrobial Activity of Restorative Materials
Standard strains of Streptococcus mutans (MTCC 497) in the form of lyophilized culture were obtained (Institute of Microbial Technology, IMTECH, Chandigarh) and used to test the antimicrobial efficacy of three different restorative materials.These microorganisms were grown in 5ml of Brain Heart infusion broth (Hi Media Laboratory Pvt. Ltd., Mumbai, India) for 24 hours at 370c to form an inoculum. The bacterial colonies were taken from the broth cultures and adjusted to 0.5 Mc Farland standard. Brain heart infusion agar was used for diffusion test. About 15ml of Brain heart infusion agar was spread evenly to a thickness of 5mm in petridish and after solidification, the agar plates were dried and three wells of 5mm diameter and 2mm depth were made in agar plate with agarpunchers. These wells were incorporated with material discs of same dimensions of three restorative materials. About 100µl of bacterial inoculum was poured with micropipette over the agar plate and it was spread evenly using plate spreader to ensure even distribution of the bacterial inoculums. All the procedures were carried out under aseptic conditions in a laminar airflow chamber. Three different materials were tested in each plate at required distances from the edge of the plate and between each other and the plates were inverted and incubated aerobically for 24 hours at 370c under 5-10% CO2.The diameter of the zones of inhibition in millimeters (mm) around the material discs were measured after 24 hours. The results were expressed as mean diameters and standard deviations.
Statistical analysis Data was analysed by one-way ANOVA (using software SPSS version 10.0) with LSD post-hoc test to compare the statistical difference of antibacterial effects in between three restorative materials tested with a bacterial strain (Streptococcus mutans).
Results The mean values and the standard deviations of the growth inhibition zones of three restorative materials are shown in [Table/Fig-1]. Intergroup comparisons in between three restorative materials by least square difference (LSD) post-hoc test are shown in [Table/Fig-2]. The post-hoc test indicated that the difference in inhibitory zones between Fuji II LC and Beautifil, Fuji II LC and F2000 showed significance (p 0.05). Materials
Mean values of inhibition zones ± SD (in mm)
Fuji II LC
10.1 ± 1.97
8.20 ± 1.62
6.90 ± 1.29
p < 0.001***
[Table/Fig-1]: Mean values of inhibition zones in mm of three restorative materials against S.mutans ***:Highly Significant (p